Journal of Nuclear Materials 455 (2014) 16–20
Contents lists available at ScienceDirect
Journal of Nuclear Materials journal homepage: www.elsevier.com/locate/jnucmat
Spatial ordering of nano-dislocation loops in ion-irradiated materials S.L. Dudarev a,⇑, K. Arakawa b, X. Yi a,c, Z. Yao d, M.L. Jenkins c, M.R. Gilbert a, P.M. Derlet e a
EURATOM/CCFE Fusion Association, Culham Centre for Fusion Energy, Oxfordshire OX14 3DB, UK Department of Materials Science, Faculty of Science and Engineering, Shimane University, 1060 Nishikawatsu, Matsue 690-8504, Japan c Department of Materials, University of Oxford, Parks Road, Oxford OX1 3PH, UK d Department of Mechanical and Materials Engineering, Queen’s University, Nicol Hall, 60 Union Street, Kingston K7L 3N6, Ontario, Canada e Condensed Matter Theory Group, Paul Scherrer Institut, CH-5232 Villigen PSI, Switzerland b
a r t i c l e
i n f o
Article history: Available online 6 March 2014
a b s t r a c t Defect microstructures formed in ion-irradiated metals, for example iron or tungsten, often exhibit patterns of spatially ordered nano-scale dislocation loops. We show that such ordered dislocation loop structures may form spontaneously as a result of Brownian motion of loops, biased by the angular-dependent elastic interaction between the loops. Patterns of spatially ordered loops form once the local density of loops produced by ion irradiation exceeds a critical threshold value. Ó 2014 EURATOM/CCFE Fusion Association. Published by Elsevier B.V. All rights reserved.
The use of ion irradiation experiments for simulating effects of neutron damage in materials has recently attracted renewed interest , stimulated by practical advantages of the method, where a relatively high irradiation dose can be accumulated over only several hours of exposure to an ion beam, as opposed to several months or years of exposure typically associated with a neutron irradiation experiment. Ion irradiation has another advantage that the relatively low energy ions, as opposed to neutrons, do not initiate nuclear reactions and do not produce unstable radioactive isotopes during irradiation, hence not making the specimens radioactive. The drawbacks associated with ion irradiation tests are (i) the small (micron) depth of penetration of ions into the material, requiring application of micro-mechanical methods for the investigation of mechanical properties of ion-irradiated samples, (ii) the proximity of surfaces, (iii) the fact that primary knock-on atom recoil spectra associated with ion impacts differ from recoil spectra generated by neutrons, and (iv) the high irradiation dose rate. The fact that dose rate signiﬁcantly inﬂuences microstructure produced in neutron-irradiation materials tests, is well documented. Materials irradiated by neutrons at high dose rate show lower swelling than the same materials irradiated to the same integral dose at a lower dose rate [2–4]. Irradiation embrittlement resulting from exposure to high-energy neutrons shows remarkable sensitivity to the dose rate, too, see for example Fig. 12 from Ref. , where exposure to lower irradiation dose rate irradiation is shown to give rise to greater embrittlement. Similarly, low dose rate ion irradiation stimulates phase decomposition of Fe–Cr alloys . ⇑ Corresponding author. Tel.: +44 1235 466513; fax: +44 1235 466435. E-mail address: [email protected]
The same alloys decompose less under high dose rate ion irradiation. Given the highly non-linear nature of microstructural evolution under irradiation, the need to relate microstructure formed under ion irradiation to microstructure produced by neutron irradiation requires the development of computer models explaining the observed dose rate effects. Within a rate theory treatment, involving single-particle distribution functions and assuming locally spatially homogeneous distribution of defect species, a higher defect production rate gives rise to the higher average concentration of radiation defects, which in turn increases the relative magnitude of non-linear terms in the rate equations, in particular the terms describing recombination of vacancies and self-interstitial atom defects, or the terms describing reactions between the defects [2,4]. Elasticity effects are included in rate theory equations through mean-ﬁeld bias factors that favor absorption of self-interstitial atoms defects by edge dislocations over absorption of vacancies [7–9]. What the rate theory analysis does not normally address is the evolution of a strongly spatially heterogeneous defect microstructure that forms as a result of elastic interaction between the defects, and the treatment of which requires the use of many-particle distribution functions, or an equivalent mathematical apparatus. Elastic interactions play a particularly signiﬁcant role in the case of dislocation loops that, as opposed to vacancies, interact even in an elastically isotropic material, for example in tungsten [10,11]. In situ electron microscope examination of metals irradiated with ultra-high-energy electrons or energetic ions [12–20] shows that nano-scale defects generated by irradiation perform stochastic Brownian motion (diffusion). If the density of defects is high, diffusion becomes biased by elastic interaction between the defects.
http://dx.doi.org/10.1016/j.jnucmat.2014.02.032 0022-3115/Ó 2014 EURATOM/CCFE Fusion Association. Published by Elsevier B.V. All rights reserved.
S.L. Dudarev et al. / Journal of Nuclear Materials 455 (2014) 16–20
The sequence of frames shown in Fig. 1, and also electron microscope images of microstructure shown in Figs. 2 and 3, illustrate how interaction between the defects affects microstructural evolution. The images show that in a dense ion-irradiation-induced microstructure nano-dislocation loops are not distributed evenly, and instead they form clusters, strings, and rafts . Furthermore, in situ time-dependent electron microscope observations provide evidence that, depending on the relative position and orientation of their Burgers vectors, nano-scale dislocation loops interact through angular-dependent elastic forces, attracting or repelling each other. Simulating real-time and real-space dynamics of microstructural evolution of an irradiated material still remains an outstanding problem. The ten orders of magnitude mismatch between the nanosecond timescale accessible to a conventional molecular dynamics (MD) simulation and the 10–1000 s timescale of a typical in situ electron microscope observation often impedes meaningful quantitative analysis of experimental data. In situ electron microscope observations show that dense microstructures formed under high irradiation dose rate conditions evolve through collective events, involving several defects moving in a correlated way , and resulting in the formation of rafts of nano-scale radiation defects. While symmetry-broken solutions of reaction–diffusion rate theory equations were discussed in the past in connection with the treatment of irradiation-induced microstructures [24–28], the origin of spatial heterogeneity of rate theory solutions discussed in Refs. [24–28] was associated either with the non-linearity of rate
Fig. 2. Microstructure of ultra-high purity iron irradiated with Fe+ ions to the dose of 1 dpa at 673 K. The microstructure is formed by dislocation loops of interstitial type. The large loops seen in the micrograph have Burgers vectors of the a=2h1 1 1i type.
equations or with the anisotropy of diffusion of defects, and not with elastic interaction between the defects. In situ observations illustrated in Fig. 1 suggest that it is the interaction between radiation defects that gives rise to the formation of locally spatially ordered defect structures. Interaction between radiation defects is
Fig. 1. A sequence of time frames taken using the g ¼ 110 imaging condition at T ¼ 725 K, which shows evolution of an ensemble of interacting mobile a=2h1 1 1i prismatic dislocation loops in pure Fe. A bound conﬁguration involving two loops is formed during the time interval between 16.76 s and 18.54 s. Coherent motion of a raft of loops is seen in the frames corresponding to the 0–2.68 s time interval. An example of cooperative motion exhibited by a bound conﬁguration of several loops is seen in the frames spanning the time interval between 31.58 s and 36.78 s.
S.L. Dudarev et al. / Journal of Nuclear Materials 455 (2014) 16–20
We assume that the loop Burgers vectors are normal to the loop habit planes, i.e. ðb1 dl1 Þ ¼ 0; ðb2 dl2 Þ ¼ 0. Integration in Eq. (4) is performed over closed contours C 1 and C 2 , corresponding to the perimeters of the loops. l is the shear modulus and r is the Poisson ratio of the material. The tensor T $ ¼ T ab has the form
T ab ¼
expected to play a particularly signiﬁcant role in the limit where the density of defects is high (this was noted already by Friedel  and Eshelby ), i.e. in the limit of high irradiation dose rate. In this paper, we investigate the stochastic dynamics of interacting nano-scale dislocation loops, extending and developing a method applied earlier [22,23] to the treatment of diffusion of nano-dislocation loops with collinear Burgers vectors, and exploring the three-dimensional dynamics of interacting loops with non-collinear Burgers vectors. In particular, we apply Langevin dynamics simulations to the interpretation of collective microstructural features found through in situ electron microscope observations of irradiated materials illustrated in Figs. 1–3. Langevin dynamics simulations of interacting dislocation loops are based on solving coupled stochastic differential equations of the form a X Dab @U dr i i ¼ þ mai ðtÞ; dt kB T @r bi b
hmai ðtÞi ¼ 0; hmai ðtÞmbj ðt0 Þi ¼ 2Diab dij dðt t0 Þ;
for i ¼ 1; 2; . . . ; N. The temperature-dependent diffusion matrix Di ¼ Diab ¼ Diab ðTÞ is related to the friction matrix ci ¼ ciab ðTÞ (in dislocation dynamics c is called the drag tensor) via the ﬂuctuation– dissipation relation
Di ðTÞ ¼ kB T½ci ðTÞ1 :
Elastic interaction between the loops is given by the following equation, derived using the isotropic elasticity approximation 
l ðb1 b2 Þðdl1 dl2 Þ r 2p C 1 C 2 I I $ l þ ðb1 dl2 Þ T ðb2 dl1 Þ: 4pð1 rÞ C 1 C2
U 12 ¼
One of the signiﬁcant features characterizing the law of elastic interaction between prismatic loops (4) is its pronounced angular character, resulting in the energy of interaction depending not only on the orientation of the loop normal vectors, but also on the orientation of these vectors with respect to the vector R1 —R2 linking the centers of the loops, as illustrated in Fig. 4. Fig. 4 shows that the energy of elastic interaction plotted as a function of position of the centre of one of the loops depends sensitively not only on the relative position of the loops but also on the orientation of their Burgers vectors. Furthermore, the ﬁgure shows that this interaction between nano-dislocation loops varies on the electron-volt scale, which is not dissimilar to the scale of activation energies characterizing thermally activated migration of point defects, see e.g. Tables 1 and 2 of Ref. . Analysis performed in Ref.  already showed that elastic interaction between mobile dislocation loops and vacancy clusters can trap mobile loops on the 100 s, or longer, timescale. A similar argument applies to self-trapping of interacting loops in the ‘‘center of mass’’ frame, where two or several loops can form a bound conﬁguration and migrate as one collective entity on the timescales of seconds, minutes, or even hours. To understand the origin of this self-trapping, we estimate the characteristic conﬁnement time for a loop trapped by one of the potential wells shown in Fig. 4. The rate of escape from a potential well by diffusion can be estimated as
expðEb =kB TÞ;
where D is the loop diffusion coefﬁcient, W is the effective width of the potential well, and Eb is the effective energy barrier that a loop
Energy of interaction between loops (eV)
Fig. 3. Microstructure of 99.95 wt% purity tungsten irradiated with 2 MeV W+ ions to the dose of 3:3 1017 Wþ =m2 at 773 K. Incident ion beam direction is close to the surface normal, which is parallel to the [1 1 3] crystallographic direction. Electron imaging condition. The microscope observations were performed using the g ¼ 121 loops that contribute to the formation of strings are of the 1=2h1 1 1i interstitial type.
@2r r 2 dab r a r b ¼ : a b @r @r r3
0.3 0.2 0.1 0 -0.1 b1=a/2[1,1,1] b1=a/2[-1,1,1]
-0.2 -0.3 -0.4 -400
displacement of loop 2 along its glide cylinder (Angstrom) Fig. 4. Energy of interaction between two dislocations loops in Fe plotted as a function of the relative position of the loops in real space for the two orientations of the Burgers vector of the ﬁrst loop, which is situated at the origin of the Cartesian system of coordinates R1 ¼ 0. The energy of interaction, computed in the isotropic elasticity approximation, is shown as a function of the position of loop 2, which has Burgers vector b2 ¼ a=2½1 1 1, along its glide cylinder. The glide direction of this loop intersects the ðx; yÞ plane at ðx; yÞ ¼ ð60; 60Þ Å. The loop radii are q1 ¼ q2 ¼ 15 Å. Values of the shear modulus l ¼ 82 GPa (in atomic units 3 l ¼ 0:511 eV=Å ) and the Poisson ratio r ¼ 0:29 for iron are taken from Appendix 1 of Ref. . Open circles represent interaction energies computed numerically using the double integral expression (4), lines correspond to a simpliﬁed analytical expression for the interaction energy.
S.L. Dudarev et al. / Journal of Nuclear Materials 455 (2014) 16–20
needs to overcome to escape from the potential well. We assume that the width of the potential well is W 20 nm (this corresponds to the collinear orientation of Burgers vectors of the loops in Fig. 4), and that the diffusion coefﬁcient DðTÞ is given by equation [23,32] DðTÞ ¼ ðD=2qÞ expðEa =kB TÞ, where D ¼ 5:7 1013 ðnmÞ3 =s, q is the loop radius (in nm units), Ea ¼ 1:3 eV is the activation energy for loop migration, and Eb 0:4 eV (this again corresponds to the collinear Burgers vectors of loops in Fig. 4). Using Eq. (6), we ﬁnd that the lifetime s ¼ 1=C of a self-trapped loop conﬁguration at various temperatures is s 3 s for T ¼ 500 C, s 130 s for T ¼ 400 C, and s 2:2 104 s (or, in other words, s 6:25 h) for T ¼ 300 C. These estimated reaction–diffusion timescales are broadly similar with what is observed experimentally, see for example Fig. 1, and other studies exploring the dynamics of migration of nano-dislocation loops in ion-irradiated iron  and tungsten . The estimates for elastic self-trapping timescales given above involve diffusion coefﬁcients for migrating loops derived from experimental observations of Brownian motion of the loops . The activation energy Ea ¼ 1:3 eV characterizing Brownian motion of loops seen experimentally is much higher than the activation energy 0:024 eV found in molecular dynamics simulations of defects in pure iron . To ﬁnd out whether impurities are responsible for the difference, we use an equation  that relates the concentration of impurities c, in atom per site units, near a defect (for example a dislocation loop) to their concentration c0 far away from a defect,
c0 exp kUB T h i: c¼ 1 þ c0 exp kUB T 1
Here U is the energy of interaction between an impurity and a defect and T is the absolute temperature. For c0 ¼ 106 , U ¼ 0:66 eV (the energy of interaction between an edge dislocation and a carbon atom in bcc iron ) and T ¼ 500 K, we ﬁnd that c 0:82. In other words, in thermodynamic equilibrium carbon impurities form a dense atmosphere around a dislocation loop even if the average concentration of carbon atoms in iron is as low as c0 ¼ 106 ¼ 1 appm. This shows that Langevin dynamics simulations, describing evolving defect conﬁgurations in the long time scale limit, should necessarily use dislocation mobilities that take into account the effect of impurity atmospheres. Among various orientations of the loops’ Burgers vectors, the collinear conﬁgurations exhibit the highest binding energy, and also the width of the potential wells describing elastic interaction between the loops is the largest in the collinear case. Noting this fact and relating it to Eq. (6), we arrive at a conclusion that an ensemble of the initially randomly distributed mobile interacting dislocation loops should exhibit a tendency towards local ordering, where loops with collinear Burgers vectors form collective relatively stable raft-like conﬁgurations. This hypothesis is conﬁrmed by direct simulations, where we analyze solutions of Langevin dynamics Eq. (1) for a large ensemble of migrating nano-dislocation loops. We ﬁnd that loops with collinear Burgers vectors do form bound conﬁgurations, which remain stable over fairly long intervals of time, whereas the loops with non-collinear Burgers vectors do not exhibit any pronounced tendency towards selfconﬁnement and spatial ordering. Fig. 5 illustrates a typical behavior of an ensemble of interacting nano-dislocation loops, evolving according to Eq. (1). The evolution of the system is conservative in the sense that the total number of self-interstitial atoms forming the loops (or, in other words, the total area of the loops) remains constant throughout the simulation. We see that the evolution of the system is continuous, and no stationary steady-state is reached on the timescale of the simulation. This is fundamentally consistent with the diffusive nature of
Fig. 5. Snapshots illustrating evolution of an ensemble of interacting nanodislocation loops simulated using the Langevin dynamics Eq. (1). The loops are initially distributed randomly in a planar slab of Fe, treated as an elastically isotropic medium. The loops are conﬁned between the two ð0 1 1Þ-type planes, to mimic a foil bound by the ð0 1 1Þ-type surfaces. No periodic boundary conditions are applied; the viewing direction is normal to the slab surface. The loop radii are chosen at random in the interval between 1 nm and 5 nm, and the loop Burgers and a=2½111. The loops interact vectors bi are chosen randomly between a=2½111 according to Eq. (4), where the shear modulus l ¼ 82 109 Pa (in atomic units 3 l ¼ 0:511 eV=Å ) and the Poisson ratio r ¼ 0:29 are taken from Appendix 1 of Ref. . The temperature of the system is T ¼ 670 K. The top panel shows the initial conﬁguration of the system, the bottom panel represents a conﬁguration formed after approximately 40 s. Note the spontaneous formation of quasi-stable string structures formed by loops with collinear Burgers vectors.
evolution where, because of the thermal noise, there is no possibility of arriving at a steady-state conﬁguration of the system. Simulations show the spontaneous formation of locally spatially ordered many-body collective loop structures, involving loops with collinear Burgers vectors, which remain stable over long intervals of time. These conﬁgurations form spontaneously in the simulations, similarly to how they form in in situ observations, see Fig. 1. The collective loop conﬁgurations eventually decay as a
S.L. Dudarev et al. / Journal of Nuclear Materials 455 (2014) 16–20
result of loops escaping by diffusion from the action of elastic forces holding them together. In agreement with the qualitative argument given in the preceding paragraph, the 3D Langevin dynamics simulations show that such a self-organization effect, namely the formation of collective loop raft structures, only involves loops with collinear Burgers vectors. This is consistent with the analysis of the Burgers vector content of loop rafts observed experimentally. The effect of formation of rafts, resulting from the combined action of elastic forces and Brownian motion of loops, is ultimately related to the fact that the density of loops is sufﬁciently high. Only in the limit of high density of defects, where the average distance between clusters of defects, for example nano-scale dislocation loops, is small, do elastic interactions play a signiﬁcant part. This highlights the need to include the treatment of elastic interactions between radiation defects in the models for microstructures formed in ion irradiation experiments, where the high dose rate of irradiation produces high densities of defects. Also, the above analysis shows that interaction and reactions between radiation defects should be expected to drive microstructural evolution towards the formation of complex self-organized conﬁgurations and microstructural instabilities – the investigation of which deserves greater effort, focused on unraveling the link between the microscopic laws of interaction between radiation defects and visible macroscopic manifestations of radiation damage. Acknowledgments The authors gratefully acknowledge discussions with A.A. Semenov, C.H. Woo, S.J. Zinkle, E. Clouet, F. Legoll, and N. Ghoniem. This work was part-funded by the RCUK Energy Programme (Grant Number EP/I501045) and by the European Union’s Horizon 2020 research and innovation programme. To obtain further information on the data and models underlying this paper please contact [email protected]
The views and opinions expressed herein do not necessarily reﬂect those of the European Commission. This work was also part-funded by the United Kingdom Engineering and Physical Sciences Research Council via a programme grant EP/G050031. We acknowledge support from Grant-in-Aid for Scientiﬁc Research (Grants Nos. 24360395, 24656371, 24560805 and 22224012) from the Ministry of Education, Sports, Culture, Science and Technology in Japan, CREST, Japan Science and Technology Agency, and Nippon Steel & Sumitomo Metal Co. Research Promotion Grant. We acknowledge support from Argonne National Laboratory (US) and the National Ion Beam Center (UK) where ion beam irradiation experiments were performed.
References  M. Kirk, M. Li, P. Baldo, Microsc Microanal 15 (Suppl. S2) (2009) 1348–1349.  T. Okita, T. Sato, N. Sekimura, F.A. Garner, L.R. Greenwood, J. Nucl. Mater. 307– 311 (2002) 322.  F.A. Garner, D.S. Gelles, L.R. Greenwood, T. Okita, N. Sekimura, W.G. Wolfer, J. Nucl. Mater. 329–333 (2004) 1008.  T. Okita, T. Sato, N. Sekimura, T. Iwai, F.A. Garner, J. Nucl. Mater. 367–370 (2007) 930–934.  A.D. Amayev, A.M. Kryukov, V.I. Levit, M.A. Sokolov, Radiation stability of VVER-440 vessel materials, in: L.E. Steele (Ed.), Radiation Embrittlement of Nuclear Reactor Pressure Vessel Steels: An International Review, ASTM STP 1170, ASTM, Philadelphia, 1993, pp. 9–29.  C.D. Hardie, C.A. Williams, S. Xu, S.G. Roberts, J. Nucl. Mater. 439 (2013) 33.  A.D. Brailsford, R. Bullough, Philos. Trans. R. Soc. London 302 (1981) 87.  C.H. Woo, J. Nucl. Mater. 98 (1981) 279.  W.G. Wolfer, J. Comput.-Aided Mater. Des. 14 (2007) 403.  J.D. Eshelby, Acta Metall. 3 (1955) 487.  T.S. Hudson, S.L. Dudarev, M.-J. Caturla, A.P. Sutton, Philos. Mag. 85 (2005) 661.  K. Arakawa, M. Hatanaka, E. Kuramoto, K. Ono, H. Mori, Phys. Rev. Lett. 96 (2006) 125506.  K. Arakawa, K. Ono, M. Isshiki, K. Mimura, M. Uchikoshi, H. Mori, Science 318 (2007) 956.  K. Arakawa, K. Ono, H. Mori, in: A. Avilov et al. (Eds.), Electron Microscopy and Multiscale Modelling, EMMM-2007, AIP Conf. Proc. No. CP999, AIP, New York, 2008, pp. 66–78.  Z. Yao, M. Hernández-Mayoral, M.L. Jenkins, M.A. Kirk, Philos. Mag. 88 (2008) 2851.  M. Hernández-Mayoral, Z. Yao, M.L. Jenkins, M.A. Kirk, Philos. Mag. 88 (2008) 2881.  M.L. Jenkins, Z. Yao, M. Hernández-Mayoral, M.A. Kirk, J. Nucl. Mater. 389 (2009) 197.  Z. Yao, M.L. Jenkins, M. Hernández-Mayoral, M.A. Kirk, Philos. Mag. 90 (2010) 4623.  K. Arakawa, T. Amino, H. Mori, Acta Mater. 59 (2011) 141.  X. Yi, M.L. Jenkins, M. Briceño, S.G. Roberts, Z. Zhou, M.A. Kirk, Philos. Mag. 93 (2013) 1715.  S.J. Zinkle, B.N. Singh, J. Nucl. Mater. 351 (2006) 269.  S.L. Dudarev, M.R. Gilbert, K. Arakawa, H. Mori, Z. Yao, M.L. Jenkins, P.M. Derlet, Phys. Rev. B 81 (2010) 224107.  P.M. Derlet, M.R. Gilbert, S.L. Dudarev, Phys. Rev. B 84 (2011) 134109.  N.M. Ghoniem, D. Walgraef, S.J. Zinkle, J. Comput.-Aided Mater. Des. 8 (2002) 1.  C.H. Woo, W. Frank, J. Nucl. Mater. 137 (1985) 7.  A.A. Semenov, C.H. Woo, Appl. Phys. A 73 (2001) 371.  A.A. Semenov, C.H. Woo, Appl. Phys. A84 (2006) 261.  A.A. Semenov, C.H. Woo, Phys. Rev. B74 (2006) 024108.  J. Friedel, Adv. Phys. 3 (1954) 446.  J.P. Hirth, J. Lothe, Theory of Dislocations, Krieger, Malabar, Florida, 1992.  S.L. Dudarev, Annu. Rev. Mater. Res. 43 (2013) 35.  Derived using an argument that the diffusion coefﬁcient is inversely proportional to the friction coefﬁcient, which is in turn proportional to the perimeter of the loop.  Y.N. Osetsky, D.J. Bacon, A. Serra, B.N. Singh, S.I. Golubov, Philos. Mag. 83 (2003) 61.  E. Clouet, S. Garruchet, H. Nguyen, M. Perez, C.S. Becquart, Acta Mater. 56 (2008) 3450.